General

Property | Temperature | Value |
---|---|---|

Density | 20.0 °C | 7.96 - 8 g/cm³ Show Material materials with Density of 7.96 - 8 g/cm³ |

22.0 °C | 7.96 g/cm³ Show Material materials with Density of 7.96 g/cm³ | |

Mechanical

Property | Temperature | Value |
---|---|---|

Elastic modulus | -100.0 °C | 206 GPa Show Material materials with Elastic modulus of 206 GPa |

20.0 °C | 196 - 200 GPa Show Material materials with Elastic modulus of 196 - 200 GPa | |

22.0 °C | 196.2 GPa Show Material materials with Elastic modulus of 196.2 GPa | |

24.0 °C | 193.1 - 197.9 GPa Show Material materials with Elastic modulus of 193.1 - 197.9 GPa | |

100.0 °C | 190 - 194 GPa Show Material materials with Elastic modulus of 190 - 194 GPa | |

149.0 °C | 184.8 - 190.3 GPa Show Material materials with Elastic modulus of 184.8 - 190.3 GPa | |

200.0 °C | 182 - 186 GPa Show Material materials with Elastic modulus of 182 - 186 GPa | |

260.0 °C | 182 - 182.7 GPa Show Material materials with Elastic modulus of 182 - 182.7 GPa | |

300.0 °C | 174 - 179 GPa Show Material materials with Elastic modulus of 174 - 179 GPa | |

371.0 °C | 174.4 - 179.3 GPa Show Material materials with Elastic modulus of 174.4 - 179.3 GPa | |

400.0 °C | 166 - 172 GPa Show Material materials with Elastic modulus of 166 - 172 GPa | |

483.0 °C | 163.4 - 165.5 GPa Show Material materials with Elastic modulus of 163.4 - 165.5 GPa | |

500.0 °C | 158 - 165 GPa Show Material materials with Elastic modulus of 158 - 165 GPa | |

593.0 °C | 153.4 - 157.9 GPa Show Material materials with Elastic modulus of 153.4 - 157.9 GPa | |

600.0 °C | 150 GPa Show Material materials with Elastic modulus of 150 GPa | |

700.0 °C | 142 GPa Show Material materials with Elastic modulus of 142 GPa | |

704.0 °C | 143.4 - 146.2 GPa Show Material materials with Elastic modulus of 143.4 - 146.2 GPa | |

800.0 °C | 134 GPa Show Material materials with Elastic modulus of 134 GPa | |

816.0 °C | 124.1 - 133.1 GPa Show Material materials with Elastic modulus of 124.1 - 133.1 GPa | |

900.0 °C | 127 GPa Show Material materials with Elastic modulus of 127 GPa | |

1000.0 °C | 120 GPa Show Material materials with Elastic modulus of 120 GPa | |

Unlock all property charts | ||

Elongation A80, transverse | 20.0 °C | 40 - 45 % Show Material materials with Elongation A80, transverse of 40 - 45 % |

Elongation, transverse | 20.0 °C | 40 - 45 % Show Material materials with Elongation, transverse of 40 - 45 % |

Poisson's ratio | 22.0 °C | 0.29 [-] Show Material materials with Poisson's ratio of 0.29 [-] |

24.0 °C | 0.23 - 0.28 [-] Show Material materials with Poisson's ratio of 0.23 - 0.28 [-] | |

149.0 °C | 0.24 - 0.28 [-] Show Material materials with Poisson's ratio of 0.24 - 0.28 [-] | |

260.0 °C | 0.28 - 0.31 [-] Show Material materials with Poisson's ratio of 0.28 - 0.31 [-] | |

371.0 °C | 0.33 - 0.36 [-] Show Material materials with Poisson's ratio of 0.33 - 0.36 [-] | |

483.0 °C | 0.29 - 0.32 [-] Show Material materials with Poisson's ratio of 0.29 - 0.32 [-] | |

593.0 °C | 0.32 [-] Show Material materials with Poisson's ratio of 0.32 [-] | |

704.0 °C | 0.28 - 0.34 [-] Show Material materials with Poisson's ratio of 0.28 - 0.34 [-] | |

816.0 °C | 0.22 - 0.27 [-] Show Material materials with Poisson's ratio of 0.22 - 0.27 [-] | |

Unlock all property charts | ||

Shear modulus | 22.0 °C | 75.8 GPa Show Material materials with Shear modulus of 75.8 GPa |

24.0 °C | 77.2 - 78.6 GPa Show Material materials with Shear modulus of 77.2 - 78.6 GPa | |

149.0 °C | 74.5 GPa Show Material materials with Shear modulus of 74.5 GPa | |

260.0 °C | 69.6 - 71 GPa Show Material materials with Shear modulus of 69.6 - 71 GPa | |

371.0 °C | 64.1 - 67.6 GPa Show Material materials with Shear modulus of 64.1 - 67.6 GPa | |

483.0 °C | 62.1 - 64.1 GPa Show Material materials with Shear modulus of 62.1 - 64.1 GPa | |

593.0 °C | 57.9 - 60 GPa Show Material materials with Shear modulus of 57.9 - 60 GPa | |

704.0 °C | 54.5 - 55.9 GPa Show Material materials with Shear modulus of 54.5 - 55.9 GPa | |

816.0 °C | 51 - 52.4 GPa Show Material materials with Shear modulus of 51 - 52.4 GPa | |

Unlock all property charts | ||

Tensile strength | 20.0 °C | 520 - 680 MPa Show Material materials with Tensile strength of 520 - 680 MPa |

50.0 °C | 486 MPa Show Material materials with Tensile strength of 486 MPa | |

100.0 °C | 430 MPa Show Material materials with Tensile strength of 430 MPa | |

150.0 °C | 410 MPa Show Material materials with Tensile strength of 410 MPa | |

200.0 °C | 390 MPa Show Material materials with Tensile strength of 390 MPa | |

250.0 °C | 385 MPa Show Material materials with Tensile strength of 385 MPa | |

300.0 °C | 380 MPa Show Material materials with Tensile strength of 380 MPa | |

350.0 °C | 380 MPa Show Material materials with Tensile strength of 380 MPa | |

Unlock all property charts | ||

Tensile strength, transverse | 20.0 °C | 520 - 680 MPa Show Material materials with Tensile strength, transverse of 520 - 680 MPa |

Yield strength Rp0.2 | 50.0 °C | 204 MPa Show Material materials with Yield strength Rp0.2 of 204 MPa |

100.0 °C | 177 MPa Show Material materials with Yield strength Rp0.2 of 177 MPa | |

150.0 °C | 162 MPa Show Material materials with Yield strength Rp0.2 of 162 MPa | |

200.0 °C | 147 MPa Show Material materials with Yield strength Rp0.2 of 147 MPa | |

250.0 °C | 137 MPa Show Material materials with Yield strength Rp0.2 of 137 MPa | |

300.0 °C | 127 MPa Show Material materials with Yield strength Rp0.2 of 127 MPa | |

350.0 °C | 120 MPa Show Material materials with Yield strength Rp0.2 of 120 MPa | |

400.0 °C | 115 MPa Show Material materials with Yield strength Rp0.2 of 115 MPa | |

450.0 °C | 112 MPa Show Material materials with Yield strength Rp0.2 of 112 MPa | |

500.0 °C | 110 MPa Show Material materials with Yield strength Rp0.2 of 110 MPa | |

550.0 °C | 108 MPa Show Material materials with Yield strength Rp0.2 of 108 MPa | |

Unlock all property charts | ||

Yield strength Rp0.2, transverse | 20.0 °C | 220 - 240 MPa Show Material materials with Yield strength Rp0.2, transverse of 220 - 240 MPa |

Yield strength Rp1.0 | 50.0 °C | 242 MPa Show Material materials with Yield strength Rp1.0 of 242 MPa |

100.0 °C | 211 MPa Show Material materials with Yield strength Rp1.0 of 211 MPa | |

150.0 °C | 191 MPa Show Material materials with Yield strength Rp1.0 of 191 MPa | |

200.0 °C | 177 MPa Show Material materials with Yield strength Rp1.0 of 177 MPa | |

250.0 °C | 167 MPa Show Material materials with Yield strength Rp1.0 of 167 MPa | |

300.0 °C | 156 MPa Show Material materials with Yield strength Rp1.0 of 156 MPa | |

350.0 °C | 150 MPa Show Material materials with Yield strength Rp1.0 of 150 MPa | |

400.0 °C | 144 MPa Show Material materials with Yield strength Rp1.0 of 144 MPa | |

450.0 °C | 141 MPa Show Material materials with Yield strength Rp1.0 of 141 MPa | |

500.0 °C | 139 MPa Show Material materials with Yield strength Rp1.0 of 139 MPa | |

550.0 °C | 137 MPa Show Material materials with Yield strength Rp1.0 of 137 MPa | |

Unlock all property charts | ||

Yield strength Rp1.0, transverse | 20.0 °C | 260 - 270 MPa Show Material materials with Yield strength Rp1.0, transverse of 260 - 270 MPa |

Thermal

Property | Temperature | Value | Comment |
---|---|---|---|

Coefficient of thermal expansion | -100.0 °C | 1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K | |

20.0 °C | 1.61E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.61E-5 1/K | ||

100.0 °C | 1.6E-5 - 1.67E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.6E-5 - 1.67E-5 1/K | ||

200.0 °C | 1.65E-5 - 1.72E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.65E-5 - 1.72E-5 1/K | ||

300.0 °C | 1.7E-5 - 1.77E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.7E-5 - 1.77E-5 1/K | ||

400.0 °C | 1.75E-5 - 1.81E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.75E-5 - 1.81E-5 1/K | ||

500.0 °C | 1.8E-5 - 1.84E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.8E-5 - 1.84E-5 1/K | ||

600.0 °C | 1.88E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.88E-5 1/K | ||

700.0 °C | 1.91E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.91E-5 1/K | ||

800.0 °C | 1.94E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.94E-5 1/K | ||

900.0 °C | 1.97E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.97E-5 1/K | ||

1000.0 °C | 2E-5 1/K Show Material materials with Coefficient of thermal expansion of 2E-5 1/K | ||

Unlock all property charts | |||

Max service temperature, long | 0 - 300 °C Show Material materials with Max service temperature, long of 0 - 300 °C | ||

Melting point | 1230 - 1480 °C Show Material materials with Melting point of 1230 - 1480 °C | Typical for Austenitic Stainless Steel | |

Specific heat capacity | -100.0 °C | 440 J/(kg·K) Show Material materials with Specific heat capacity of 440 J/(kg·K) | |

20.0 °C | 472 - 500 J/(kg·K) Show Material materials with Specific heat capacity of 472 - 500 J/(kg·K) | ||

100.0 °C | 487 J/(kg·K) Show Material materials with Specific heat capacity of 487 J/(kg·K) | ||

200.0 °C | 503 J/(kg·K) Show Material materials with Specific heat capacity of 503 J/(kg·K) | ||

300.0 °C | 512 J/(kg·K) Show Material materials with Specific heat capacity of 512 J/(kg·K) | ||

400.0 °C | 520 J/(kg·K) Show Material materials with Specific heat capacity of 520 J/(kg·K) | ||

500.0 °C | 530 J/(kg·K) Show Material materials with Specific heat capacity of 530 J/(kg·K) | ||

600.0 °C | 541 J/(kg·K) Show Material materials with Specific heat capacity of 541 J/(kg·K) | ||

700.0 °C | 551 J/(kg·K) Show Material materials with Specific heat capacity of 551 J/(kg·K) | ||

800.0 °C | 559 J/(kg·K) Show Material materials with Specific heat capacity of 559 J/(kg·K) | ||

900.0 °C | 565 J/(kg·K) Show Material materials with Specific heat capacity of 565 J/(kg·K) | ||

1000.0 °C | 571 J/(kg·K) Show Material materials with Specific heat capacity of 571 J/(kg·K) | ||

Unlock all property charts | |||

Thermal conductivity | 20.0 °C | 13.3 - 15 W/(m·K) Show Material materials with Thermal conductivity of 13.3 - 15 W/(m·K) | |

100.0 °C | 14.9 W/(m·K) Show Material materials with Thermal conductivity of 14.9 W/(m·K) | ||

200.0 °C | 16.5 W/(m·K) Show Material materials with Thermal conductivity of 16.5 W/(m·K) | ||

300.0 °C | 18.1 W/(m·K) Show Material materials with Thermal conductivity of 18.1 W/(m·K) | ||

400.0 °C | 19.5 W/(m·K) Show Material materials with Thermal conductivity of 19.5 W/(m·K) | ||

500.0 °C | 21 W/(m·K) Show Material materials with Thermal conductivity of 21 W/(m·K) | ||

600.0 °C | 22.4 W/(m·K) Show Material materials with Thermal conductivity of 22.4 W/(m·K) | ||

700.0 °C | 23.8 W/(m·K) Show Material materials with Thermal conductivity of 23.8 W/(m·K) | ||

800.0 °C | 25.2 W/(m·K) Show Material materials with Thermal conductivity of 25.2 W/(m·K) | ||

Unlock all property charts | |||

Thermal diffusivity | 20.0 °C | 3.5 mm²/s Show Material materials with Thermal diffusivity of 3.5 mm²/s | |

100.0 °C | 3.8 mm²/s Show Material materials with Thermal diffusivity of 3.8 mm²/s | ||

200.0 °C | 4 mm²/s Show Material materials with Thermal diffusivity of 4 mm²/s | ||

300.0 °C | 4.3 mm²/s Show Material materials with Thermal diffusivity of 4.3 mm²/s | ||

400.0 °C | 4.5 mm²/s Show Material materials with Thermal diffusivity of 4.5 mm²/s | ||

500.0 °C | 4.7 mm²/s Show Material materials with Thermal diffusivity of 4.7 mm²/s | ||

600.0 °C | 4.8 mm²/s Show Material materials with Thermal diffusivity of 4.8 mm²/s | ||

700.0 °C | 5.1 mm²/s Show Material materials with Thermal diffusivity of 5.1 mm²/s | ||

800.0 °C | 5.4 mm²/s Show Material materials with Thermal diffusivity of 5.4 mm²/s | ||

Unlock all property charts |

Electrical

Property | Temperature | Value |
---|---|---|

Electrical resistivity | 20.0 °C | 7.5E-7 - 7.91E-7 Ω·m Show Material materials with Electrical resistivity of 7.5E-7 - 7.91E-7 Ω·m |

100.0 °C | 8.45E-7 Ω·m Show Material materials with Electrical resistivity of 8.45E-7 Ω·m | |

200.0 °C | 9.19E-7 Ω·m Show Material materials with Electrical resistivity of 9.19E-7 Ω·m | |

300.0 °C | 9.77E-7 Ω·m Show Material materials with Electrical resistivity of 9.77E-7 Ω·m | |

400.0 °C | 1.03E-6 Ω·m Show Material materials with Electrical resistivity of 1.03E-6 Ω·m | |

500.0 °C | 1.08E-6 Ω·m Show Material materials with Electrical resistivity of 1.08E-6 Ω·m | |

600.0 °C | 1.12E-6 Ω·m Show Material materials with Electrical resistivity of 1.12E-6 Ω·m | |

700.0 °C | 1.15E-6 Ω·m Show Material materials with Electrical resistivity of 1.15E-6 Ω·m | |

800.0 °C | 1.18E-6 Ω·m Show Material materials with Electrical resistivity of 1.18E-6 Ω·m | |

Unlock all property charts |

Chemical properties

Property | Value |
---|---|

Carbon | 0.07 % Show Material materials with Carbon of 0.07 % |

Chromium | 16.5 - 18.5 % Show Material materials with Chromium of 16.5 - 18.5 % |

Manganese | 2 % Show Material materials with Manganese of 2 % |

Molybdenum | 2 - 2.5 % Show Material materials with Molybdenum of 2 - 2.5 % |

Nickel | 10 - 13 % Show Material materials with Nickel of 10 - 13 % |

Nitrogen | 0.1 - 0.11 % Show Material materials with Nitrogen of 0.1 - 0.11 % |

Phosphorus | 0.05 % Show Material materials with Phosphorus of 0.05 % |

Silicon | 1 % Show Material materials with Silicon of 1 % |

Sulfur | 0.015 % Show Material materials with Sulfur of 0.015 % |